Chapter 14 Carbon and Alloy SteelsAll of these steels are alloys of Fe and CPlain carbon steels (less than 2% carbon and negligible amounts of other residual elements)Low Carbon (less than 0.3% carbon)Med Carbon (0.3% to 0.6%)High Carbon (0.6% to 0.95%)Low Alloy SteelHigh Alloy SteelStainless Steels (Corrosion-Resistant Steels) contain at least 10.5% Chromium
AISI - SAE Classification System AISI XXXXAmerican Iron and Steel Institute (AISI)classifies alloys by chemistry4 digit number1st number is the major alloying element2nd number designates the subgroup alloying element OR the relative percent of primary alloying element.last two numbers approximate amount of carbon (expresses in 0.01%)
Common Carbon and Alloy Steels:
AISI - SAE Classification Systemletter prefix to designate the process used to produce the steelE = electric furnaceX = indicates permissible variationsIf a letter is inserted between the 2nd and 3rd numberB = boron has been addedL = lead has been addedLetter suffixH = when hardenability is a major requirementOther designation organizationsASTM and MIL
AISI/SAE most common, also have Unified Numbering System (UNS) and ASTM
Plain Carbon SteelPlain Carbon SteelLowest cost Should be considered first in most application3 Classifications Low Carbon (less than 0.3% carbon)Med Carbon (0.3% to 0.6%)High Carbon (0.6% to 0.95%)
Plain Carbon SteelAgain, alloy of iron and carbon with carbon the major strengthening element via solid solution strengthening.If carbon level high enough (greater than 0.6%) can be quench hardened (aka: dispersion hardening, through hardened, heat treated, austenized and quenched, etc..).Can come in HRS and CRS optionsThe most common CRS are 1006 through 1050 and 1112, 1117 and other free machining steels
Low Carbon (less than 0.3% carbon)Low strength, good formabilityIf wear is a potential problem, can be carburized (diffusion hardening)Most stampings made from these steelsAISI 1008, 1010, 1015, 1018, 1020, 1022, 1025
2. Med Carbon (0.3% to 0.6%)Have moderate to high strength with fairly good ductilityCan be used in most machine elementsAISI 1030, 1040, 1050, 1060*
High Carbon (0.6% to 0.95%)Have high strength, lower elongationCan be quench hardenedUsed in applications where surface subject to abrasion tools, knives, chisels, ag implements.AISI 1080, 1095Plain Carbon Steel
Trends?Increasing carbon content tensile strength increases, elongation decreases.
Carbon steels: low, med and hight
Plain Carbon Steel1018Low carbonYield strength 55ksi1045Medium carbonYield strength 70ksiA36Low carbonYield strength 36ksi12L14Low carbonYield strength 70ksi1144Medium carbonYield strength 95ksi
HRS vs. CRSHRSAKA hot finishing ingots or continuous cast shapes rolled in the HOT condition to a smaller shape.Since hot, grains recrystallize without material getting harder!Dislocations are annihilated (recall dislocations impede slip motion).HRS Characterized by:Extremely ductile (i.e. % elongation 20 to 30%)Moderate strength (Su approx 60 75 ksi for 1020)Rough surface finish black scale left on surface.
HRS vs. CRSCRSAKA cold finishing coil of HRS rolled through a series of rolling mills AT ROOM TEMPERATURE.Since rolled at room temperature, get crystal defects called dislocations which impede motion via slip!AKA work hardeningLimit to how much you can work harden before too brittle.How reverse? Can recrystallize by annealing.CRS Characterized by:Less ductlie almost brittle (i.e. % elongation 5 to 10%)High strength (Su approx 120 ksi for 1020)
Alloy SteelOther elements (besides carbon) can be added to iron to improve mechanical property, manufacturing, or environmental property. Example: sulfur, phosphorous, or lead can be added to improve machine ability.Generally want to use for screw machine parts or parts with high production rates!Examples: 11xx, 12xx and 12Lxx
Alloy SteelAgain, elements added to steel can dissolve in iron (solid solution strengthening):Increase strength, hardenability, toughness, creep, high temp resistance.Alloy steels grouped into low, med and high-alloy steels.High-alloy steels would be the stainless steel groups.Most alloy steels youll use fall under the category of low alloy.
Alloy Steel> 1.65%Mn, > 0.60% Si, or >0.60% CuMost common alloy elements:Chromium, nickel, molybdenum, vanadium, tungsten, cobalt, boron, and copper.Low alloy: Added in small percents (20%) i.e. > 10.5% Cr = stainless steel where Cr improves corrosion resistance and stability at high or low temps
Alloying Elements used in SteelManganese (Mn)combines with sulfur to prevent brittleness>1% increases hardenability11% to 14%increases hardnessgood ductilityhigh strain hardening capacityexcellent wear resistanceIdeal for impact resisting tools
Alloying Elements used in SteelSulfur (S)Imparts brittlenessImproves machineabilityOkay if combined with MnSome free-machining steels contain 0.08% to 0.15% SExamples of S alloys:11xx sulfurized (free-cutting)
Alloying Elements used in SteelNickel (Ni)Provides strength, stability and toughness, Examples of Ni alloys:30xx Nickel (0.70%), chromium (0.70%)31xx Nickel (1.25%), chromium (0.60%)32xx Nickel (1.75%), chromium (1.00%)33XX Nickel (3.50%), chromium (1.50%)
Alloying Elements used in SteelChromium (Cr)Usually < 2% increase hardenability and strengthOffers corrosion resistance by forming stable oxide surfacetypically used in combination with Ni and Mo30XX Nickel (0.70%), chromium (0.70%)5xxx chromium alloys6xxx chromium-vanadium alloys41xxx chromium-molybdenum alloysMolybdenum (Mo)Usually < 0.3% increase hardenability and strengthMo-carbides help increase creep resistance at elevated tempstypical application is hot working tools
Alloying Elements used in SteelVanadium (V)Usually 0.03% to 0.25%increase strengthwithout loss of ductilityTungsten (W)helps to form stable carbidesincreases hot hardnessused in tool steels
Alloying Elements used in SteelCopper (Cu)0.10% to 0.50%increase corrosion resistanceReduced surface quality and hot-working abilityused in low carbon sheet steel and structural steelsSilicon (Si)About 2% increase strength without loss of ductilityenhances magnetic properties
Alloying Elements used in SteelBoron (B)for low carbon steels, can drastically increase hardenabilityimproves machinablity and cold forming capacityAluminum (Al)deoxidizer0.95% to 1.30%produce Al-nitrides during nitriding
Corrosion Resistant SteelStainless Steels (Corrosion-Resistant Steels) contain at least 10.5% Chromiumtrade nameAISI assigns a 3 digit number200 and 300 Austenitic Stainless Steel400 Ferritic or Martensitic Stainless Steel500 Martensitic Stainless Steel
Tool SteelRefers to a variety of carbon and alloy steels that are particularly well-suited to be made into tools. Characteristics include high hardness, resistance to abrasion (excellent wear), an ability to hold a cutting edge, resistance to deformation at elevated temperatures (red-hardness). Tool steel are generally used in a heat-treated state.High carbon content very brittle
AISI-SAE tool steel gradesDefining propertyAISI-SAE gradeSignificant characteristicsWater-hardeningWCold-workingOOil-hardeningAAir-hardening; medium alloyDHigh carbon; high chromiumShock resistingSHigh speedTTungsten baseMMolybdenum baseHot-workingHH1-H19: chromium base H20-H39: tungsten base H40-H59: molybdenum basePlastic moldPSpecial purposeLLow alloyFCarbon tungsten
Recall, tensile strength approximately 500 X BHN
A Quick Review of Heat Treating Processes from Chapter 13:
Know These Basic HT Processes:Full Annealing Heat above the austenite temperature (or UC) until the composition is uniform. Cool very slowly (usually at room temperate outside the oven. Result: a soft, low-strength steel, free of significant internal stresses. Generally done before Cold Forming process.Stress relief annealing Heat slightly below austenitic temperature (or below LC) generally done following welding, machining or cold forming to reduce residual stress.
Know These Basic HT Processes:Normalizing: Similar to annealing but at higher temperature. Again, slow cooling. Result: uniform internal structure with somewhat higher strength than the annealing process. Machinability and toughness improved over the as-rolled condition.
Know These Basic HT Processes:Through Hardening, Quenching and Tempering (and then slow cooling): Heat above the austenite temperature (or UC) until the composition is uniform. Cool rapidly (Quench). Result: strong but brittle martensite structure. So temper and slow cool to improve toughness at the expense of strength.
Tensile Strength and Elongation vs Tempering Temperature
Spheroidizing: (must have carbon content of 0.6% or higher) Spheroidite forms when carbon steel is heated to approximately 700C for over 30 hours. Spheroidite can form at lower temperatures but the time needed drastically increases, as this is a diffusion-controlled process. The result is a structure of rods or spheres of cementite within primary structure (ferrite or pearlite, depending on which side of the eutectoid you are on). The purpose is to soften higher carbon steels and allow more formability. This is the softest and most ductile form of steel. The image to the right shows where spheroidizing usually occurs.Know These Basic HT Processes:
HRS vs CRS vs Annealed?HT?
Tensile Strength and El